 
data_ga_200721ca_a
 
_audit_creation_method            'SHELXL-2016/6'
_shelx_SHELXL_version_number      '2016/6'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'Cs8 Mn2 Mo14 O65' 
_chemical_formula_weight          3556.32

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'Cs'  'Cs'  -0.1739   6.3004
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'  -0.0162   2.2332
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mo'  'Mo'  -0.2130   2.1496
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0389   0.0241
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       orthorhombic
_space_group_IT_number            62
_space_group_name_H-M_alt         'P n m a'
_space_group_name_Hall            '-P 2ac 2n'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x+1/2, -y, z+1/2'
 '-x, y+1/2, -z'
 'x+1/2, -y+1/2, -z+1/2'
 '-x, -y, -z'
 'x-1/2, y, -z-1/2'
 'x, -y-1/2, z'
 '-x-1/2, y-1/2, z-1/2'
 
_cell_length_a                    23.5716(17)
_cell_length_b                    10.7966(8)
_cell_length_c                    12.5938(9)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma               90
_cell_volume                      3205.0(4)
_cell_formula_units_Z             2
_cell_measurement_temperature     173(2)
_cell_measurement_reflns_used      9895
_cell_measurement_theta_min        4.47
_cell_measurement_theta_max       55.10
 
_exptl_crystal_description        block
_exptl_crystal_colour             yellow
_exptl_crystal_density_meas       3.704
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     3.685         
_exptl_crystal_F_000              3770
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.150
_exptl_crystal_size_mid           0.080
_exptl_crystal_size_min           0.060
_exptl_absorpt_coefficient_mu     41.593
_shelx_estimated_absorpt_T_min    0.032
_shelx_estimated_absorpt_T_max    0.095
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_correction_T_min   0.002
_exptl_absorpt_correction_T_max   0.012
_exptl_absorpt_process_details    SADABS
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       173(2)
_diffrn_radiation_wavelength      1.34138
_diffrn_radiation_type            GaK\a
_diffrn_source                    ?
_diffrn_measurement_device_type   'Bruker APEX-II CCD'
_diffrn_measurement_method        ?
_diffrn_detector_area_resol_mean  ?
_diffrn_reflns_number             38979
_diffrn_reflns_av_unetI/netI      0.0364
_diffrn_reflns_av_R_equivalents   0.0878
_diffrn_reflns_limit_h_min        -28
_diffrn_reflns_limit_h_max        27
_diffrn_reflns_limit_k_min        -13
_diffrn_reflns_limit_k_max        13
_diffrn_reflns_limit_l_min        -15
_diffrn_reflns_limit_l_max        15
_diffrn_reflns_theta_min          3.262
_diffrn_reflns_theta_max          55.163
_diffrn_reflns_theta_full         53.594
_diffrn_measured_fraction_theta_max   0.994
_diffrn_measured_fraction_theta_full  1.000
_diffrn_reflns_Laue_measured_fraction_max    0.994
_diffrn_reflns_Laue_measured_fraction_full   1.000
_diffrn_reflns_point_group_measured_fraction_max   0.994
_diffrn_reflns_point_group_measured_fraction_full  1.000
_reflns_number_total              3235
_reflns_number_gt                 3088
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution     'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement 'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0849P)²+175.1546P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          3235
_refine_ls_number_parameters      219
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0652
_refine_ls_R_factor_gt            0.0614
_refine_ls_wR_factor_ref          0.1764
_refine_ls_wR_factor_gt           0.1674
_refine_ls_goodness_of_fit_ref    1.089
_refine_ls_restrained_S_all       1.089
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Mo1 Mo 0.63230(6) 0.250000 0.22629(10) 0.0097(3) Uani 1 2 d S T P . .
Mo2 Mo 0.62860(4) 0.44422(9) 0.44242(8) 0.0133(3) Uani 1 1 d . . . . .
Mo3 Mo 0.52203(4) 0.44807(9) 0.27772(8) 0.0143(3) Uani 1 1 d . . . . .
Mo4 Mo 0.73052(6) 0.250000 0.41630(11) 0.0146(3) Uani 1 2 d S T P . .
Mo5 Mo 0.50971(6) 0.250000 0.09307(11) 0.0140(3) Uani 1 2 d S T P . .
Mn1 Mn 0.58569(13) 0.750000 0.3446(2) 0.0160(6) Uani 1 2 d S T P . .
Cs1 Cs 0.57627(7) 0.250000 0.72927(12) 0.0414(4) Uani 1 2 d S T P . .
Cs2 Cs 0.61580(5) -0.03525(13) 0.01071(13) 0.0593(5) Uani 1 1 d . . . . .
Cs3 Cs 0.64481(6) 0.750000 0.64537(10) 0.0315(4) Uani 1 2 d S T P . .
O1 O 0.6437(5) 0.250000 0.4080(9) 0.012(2) Uani 1 2 d S T P . .
O2 O 0.5349(5) 0.250000 0.2498(9) 0.011(2) Uani 1 2 d S T P . .
O3 O 0.7078(4) 0.4267(9) 0.4029(7) 0.0169(19) Uani 1 1 d . . . . .
O4 O 0.6162(4) 0.0876(9) 0.2649(7) 0.0149(18) Uani 1 1 d . . . . .
O5 O 0.5499(4) 0.4114(8) 0.4214(7) 0.0164(18) Uani 1 1 d . . . . .
O6 O 0.6129(6) 0.250000 0.0934(10) 0.018(3) Uani 1 2 d S T P . .
O7 O 0.5217(4) 0.4253(8) 0.1296(7) 0.0176(19) Uani 1 1 d . . . . .
O8 O 0.7054(5) 0.250000 0.2308(10) 0.017(3) Uani 1 2 d S T P . .
O9 O 0.6287(4) 0.6061(9) 0.4259(8) 0.022(2) Uani 1 1 d . . . . .
O10 O 0.6341(4) 0.4228(10) 0.5745(7) 0.023(2) Uani 1 1 d . . . . .
O11 O 0.6498(7) 0.750000 0.2176(12) 0.034(4) Uani 1 2 d S T P . .
O12 O 0.5356(4) 0.6067(9) 0.2763(7) 0.022(2) Uani 1 1 d . . . . .
O13 O 0.7415(7) 0.250000 0.5478(11) 0.025(3) Uani 1 2 d S T P . .
O14 O 0.8019(4) 0.3187(10) 0.3630(9) 0.030(2) Uani 1 1 d . . . . .
O15 O 0.4520(4) 0.4335(10) 0.3042(9) 0.030(2) Uani 1 1 d . . . . .
O16 O 0.4387(6) 0.250000 0.1078(11) 0.023(3) Uani 1 2 d S T P . .
O17 O 0.5188(5) 0.1835(11) -0.0476(8) 0.036(3) Uani 1 1 d . . . . .
O18 O 0.5227(6) 0.750000 0.4737(11) 0.023(3) Uani 1 2 d S T P . .
O19 O 0.7597(6) 0.6057(19) 0.5277(13) 0.070(5) Uani 1 1 d . . . . .
O20 O 0.7325(5) -0.0512(11) 0.2090(9) 0.035(3) Uiso 1 1 d . . . . .
O22 O 0.688(2) 0.302(5) 0.828(4) 0.046(12) Uiso 0.25 1 d . . P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Mo1 O8 1.723(13) . ?
Mo1 O6 1.734(13) . ?
Mo1 O4 1.858(9) . ?
Mo1 O4 1.858(9) 7_565 ?
Mo1 O1 2.305(11) . ?
Mo1 O2 2.314(12) . ?
Mo1 Cs2 4.1240(14) 7_565 ?
Mo1 Cs2 4.1240(14) . ?
Mo2 O10 1.684(9) . ?
Mo2 O9 1.760(10) . ?
Mo2 O5 1.908(9) . ?
Mo2 O3 1.941(9) . ?
Mo2 O1 2.171(3) . ?
Mo2 O4 2.281(8) 7_565 ?
Mo2 Mo4 3.2058(15) . ?
Mo2 Cs3 4.1925(13) . ?
Mo2 Cs1 4.3553(17) . ?
Mo3 O15 1.691(10) . ?
Mo3 O12 1.742(10) . ?
Mo3 O7 1.881(10) . ?
Mo3 O5 1.965(9) . ?
Mo3 O2 2.189(3) . ?
Mo3 O4 2.260(9) 7_565 ?
Mo3 Mo5 3.1726(14) . ?
Mo3 Cs1 4.0004(14) 5_666 ?
Mo3 Cs2 4.1326(17) 7_565 ?
Mo4 O13 1.676(13) . ?
Mo4 O14 1.957(10) 7_565 ?
Mo4 O14 1.957(10) . ?
Mo4 O3 1.989(10) . ?
Mo4 O3 1.989(10) 7_565 ?
Mo4 O1 2.049(12) . ?
Mo4 O8 2.410(12) . ?
Mo4 Cs2 4.4623(17) 8_766 ?
Mo4 Cs2 4.4622(17) 2_655 ?
Mo4 Cs3 4.503(2) 2_664 ?
Mo5 O16 1.684(14) . ?
Mo5 O17 1.923(11) 7_565 ?
Mo5 O17 1.923(11) . ?
Mo5 O7 1.968(9) . ?
Mo5 O7 1.969(9) 7_565 ?
Mo5 O2 2.061(12) . ?
Mo5 O6 2.433(13) . ?
Mo5 Cs2 3.9796(17) 5_655 ?
Mo5 Cs2 3.9796(17) 3_655 ?
Mo5 Cs2 4.1004(16) 7_565 ?
Mn1 O9 2.119(10) . ?
Mn1 O9 2.119(10) 7_575 ?
Mn1 O12 2.127(10) 7_575 ?
Mn1 O12 2.127(10) . ?
Mn1 O11 2.199(16) . ?
Mn1 O18 2.202(13) . ?
Mn1 Cs1 3.929(3) 5_666 ?
Mn1 Cs3 4.036(3) . ?
Cs1 O22 2.97(5) 7_565 ?
Cs1 O22 2.97(5) . ?
Cs1 O10 3.024(10) 7_565 ?
Cs1 O10 3.024(10) . ?
Cs1 O12 3.059(10) 3_646 ?
Cs1 O12 3.059(10) 5_666 ?
Cs1 O17 3.202(12) 7_566 ?
Cs1 O17 3.202(12) 1_556 ?
Cs1 O18 3.461(15) 5_666 ?
Cs1 O15 3.507(11) 3_646 ?
Cs1 O15 3.507(11) 5_666 ?
Cs2 O7 2.927(9) 7_565 ?
Cs2 O16 3.042(8) 5_655 ?
Cs2 O14 3.116(10) 8_755 ?
Cs2 O6 3.252(4) . ?
Cs2 O19 3.313(17) 8_755 ?
Cs2 O17 3.369(12) . ?
Cs2 O4 3.465(9) . ?
Cs2 O11 3.579(12) 1_545 ?
Cs2 O17 3.584(12) 5_655 ?
Cs2 O7 3.716(9) 3_645 ?
Cs2 O20 3.720(12) . ?
Cs3 O15 3.088(11) 5_666 ?
Cs3 O15 3.088(11) 3_656 ?
Cs3 O14 3.105(11) 8_766 ?
Cs3 O14 3.105(11) 2_665 ?
Cs3 O9 3.193(10) . ?
Cs3 O9 3.193(10) 7_575 ?
Cs3 O19 3.458(16) 7_575 ?
Cs3 O19 3.458(16) . ?
Cs3 O18 3.600(15) . ?
Cs3 O10 3.652(11) . ?
Cs3 O10 3.652(11) 7_575 ?
Cs3 O16 3.680(15) 5_666 ?
O14 O14 1.48(2) 7_565 ?
O17 O17 1.44(2) 7_565 ?
O22 O22 1.12(11) 7_565 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O8 Mo1 O6 107.2(6) . . ?
O8 Mo1 O4 101.2(3) . . ?
O6 Mo1 O4 101.5(3) . . ?
O8 Mo1 O4 101.2(3) . 7_565 ?
O6 Mo1 O4 101.5(3) . 7_565 ?
O4 Mo1 O4 141.3(5) . 7_565 ?
O8 Mo1 O1 81.4(5) . . ?
O6 Mo1 O1 171.4(5) . . ?
O4 Mo1 O1 76.3(3) . . ?
O4 Mo1 O1 76.3(3) 7_565 . ?
O8 Mo1 O2 170.8(5) . . ?
O6 Mo1 O2 82.1(5) . . ?
O4 Mo1 O2 76.4(3) . . ?
O4 Mo1 O2 76.4(3) 7_565 . ?
O1 Mo1 O2 89.4(4) . . ?
O8 Mo1 Cs2 96.7(3) . 7_565 ?
O6 Mo1 Cs2 48.70(6) . 7_565 ?
O4 Mo1 Cs2 149.0(3) . 7_565 ?
O4 Mo1 Cs2 56.5(3) 7_565 7_565 ?
O1 Mo1 Cs2 131.67(3) . 7_565 ?
O2 Mo1 Cs2 89.5(2) . 7_565 ?
O8 Mo1 Cs2 96.7(3) . . ?
O6 Mo1 Cs2 48.70(6) . . ?
O4 Mo1 Cs2 56.5(3) . . ?
O4 Mo1 Cs2 149.0(3) 7_565 . ?
O1 Mo1 Cs2 131.67(3) . . ?
O2 Mo1 Cs2 89.5(2) . . ?
Cs2 Mo1 Cs2 96.62(6) 7_565 . ?
O10 Mo2 O9 104.6(5) . . ?
O10 Mo2 O5 100.8(4) . . ?
O9 Mo2 O5 99.7(4) . . ?
O10 Mo2 O3 99.5(4) . . ?
O9 Mo2 O3 93.7(4) . . ?
O5 Mo2 O3 151.9(4) . . ?
O10 Mo2 O1 93.0(5) . . ?
O9 Mo2 O1 159.3(4) . . ?
O5 Mo2 O1 87.3(4) . . ?
O3 Mo2 O1 72.4(4) . . ?
O10 Mo2 O4 163.2(4) . 7_565 ?
O9 Mo2 O4 91.9(4) . 7_565 ?
O5 Mo2 O4 73.2(3) . 7_565 ?
O3 Mo2 O4 81.8(3) . 7_565 ?
O1 Mo2 O4 71.3(4) . 7_565 ?
O10 Mo2 Mo4 87.3(4) . . ?
O9 Mo2 Mo4 129.5(3) . . ?
O5 Mo2 Mo4 126.4(3) . . ?
O3 Mo2 Mo4 35.8(3) . . ?
O1 Mo2 Mo4 39.2(3) . . ?
O4 Mo2 Mo4 84.1(2) 7_565 . ?
O10 Mo2 Cs3 59.9(4) . . ?
O9 Mo2 Cs3 44.8(3) . . ?
O5 Mo2 Cs3 108.6(3) . . ?
O3 Mo2 Cs3 98.3(3) . . ?
O1 Mo2 Cs3 150.2(3) . . ?
O4 Mo2 Cs3 136.7(2) 7_565 . ?
Mo4 Mo2 Cs3 120.62(4) . . ?
O10 Mo2 Cs1 30.3(4) . . ?
O9 Mo2 Cs1 125.2(3) . . ?
O5 Mo2 Cs1 75.5(3) . . ?
O3 Mo2 Cs1 116.0(3) . . ?
O1 Mo2 Cs1 75.3(3) . . ?
O4 Mo2 Cs1 134.8(2) 7_565 . ?
Mo4 Mo2 Cs1 88.99(4) . . ?
Cs3 Mo2 Cs1 84.22(3) . . ?
O15 Mo3 O12 105.9(5) . . ?
O15 Mo3 O7 100.3(5) . . ?
O12 Mo3 O7 96.8(4) . . ?
O15 Mo3 O5 97.2(5) . . ?
O12 Mo3 O5 98.4(4) . . ?
O7 Mo3 O5 152.6(4) . . ?
O15 Mo3 O2 94.4(5) . . ?
O12 Mo3 O2 158.9(5) . . ?
O7 Mo3 O2 73.3(4) . . ?
O5 Mo3 O2 84.5(4) . . ?
O15 Mo3 O4 163.2(4) . 7_565 ?
O12 Mo3 O4 89.2(4) . 7_565 ?
O7 Mo3 O4 84.9(3) . 7_565 ?
O5 Mo3 O4 72.7(3) . 7_565 ?
O2 Mo3 O4 71.7(4) . 7_565 ?
O15 Mo3 Mo5 89.6(4) . . ?
O12 Mo3 Mo5 132.2(3) . . ?
O7 Mo3 Mo5 35.4(3) . . ?
O5 Mo3 Mo5 124.7(3) . . ?
O2 Mo3 Mo5 40.2(3) . . ?
O4 Mo3 Mo5 85.6(2) 7_565 . ?
O15 Mo3 Cs1 61.0(4) . 5_666 ?
O12 Mo3 Cs1 46.0(3) . 5_666 ?
O7 Mo3 Cs1 94.7(3) . 5_666 ?
O5 Mo3 Cs1 112.2(3) . 5_666 ?
O2 Mo3 Cs1 150.8(3) . 5_666 ?
O4 Mo3 Cs1 135.0(2) 7_565 5_666 ?
Mo5 Mo3 Cs1 118.69(4) . 5_666 ?
O15 Mo3 Cs2 134.7(4) . 7_565 ?
O12 Mo3 Cs2 70.7(3) . 7_565 ?
O7 Mo3 Cs2 39.2(3) . 7_565 ?
O5 Mo3 Cs2 128.1(3) . 7_565 ?
O2 Mo3 Cs2 91.0(3) . 7_565 ?
O4 Mo3 Cs2 57.0(2) 7_565 7_565 ?
Mo5 Mo3 Cs2 66.80(4) . 7_565 ?
Cs1 Mo3 Cs2 96.10(3) 5_666 7_565 ?
O13 Mo4 O14 101.9(6) . 7_565 ?
O13 Mo4 O14 101.9(6) . . ?
O14 Mo4 O14 44.6(6) 7_565 . ?
O13 Mo4 O3 97.2(3) . . ?
O14 Mo4 O3 124.5(4) 7_565 . ?
O14 Mo4 O3 80.7(4) . . ?
O13 Mo4 O3 97.2(3) . 7_565 ?
O14 Mo4 O3 80.7(4) 7_565 7_565 ?
O14 Mo4 O3 124.5(4) . 7_565 ?
O3 Mo4 O3 147.2(5) . 7_565 ?
O13 Mo4 O1 101.8(6) . . ?
O14 Mo4 O1 147.2(4) 7_565 . ?
O14 Mo4 O1 147.2(4) . . ?
O3 Mo4 O1 74.2(3) . . ?
O3 Mo4 O1 74.1(3) 7_565 . ?
O13 Mo4 O8 174.6(6) . . ?
O14 Mo4 O8 83.1(4) 7_565 . ?
O14 Mo4 O8 83.1(4) . . ?
O3 Mo4 O8 81.5(3) . . ?
O3 Mo4 O8 81.5(3) 7_565 . ?
O1 Mo4 O8 72.8(4) . . ?
O13 Mo4 Mo2 90.8(4) . . ?
O14 Mo4 Mo2 158.0(3) 7_565 . ?
O14 Mo4 Mo2 115.5(3) . . ?
O3 Mo4 Mo2 34.9(3) . . ?
O3 Mo4 Mo2 115.8(3) 7_565 . ?
O1 Mo4 Mo2 41.99(7) . . ?
O8 Mo4 Mo2 85.1(2) . . ?
O13 Mo4 Mo2 90.8(4) . 7_565 ?
O14 Mo4 Mo2 115.5(3) 7_565 7_565 ?
O14 Mo4 Mo2 158.0(3) . 7_565 ?
O3 Mo4 Mo2 115.8(3) . 7_565 ?
O3 Mo4 Mo2 34.9(3) 7_565 7_565 ?
O1 Mo4 Mo2 41.99(7) . 7_565 ?
O8 Mo4 Mo2 85.1(2) . 7_565 ?
Mo2 Mo4 Mo2 81.70(5) . 7_565 ?
O13 Mo4 Cs2 67.1(4) . 8_766 ?
O14 Mo4 Cs2 65.8(3) 7_565 8_766 ?
O14 Mo4 Cs2 36.6(3) . 8_766 ?
O3 Mo4 Cs2 75.1(2) . 8_766 ?
O3 Mo4 Cs2 137.7(3) 7_565 8_766 ?
O1 Mo4 Cs2 145.51(13) . 8_766 ?
O8 Mo4 Cs2 117.3(2) . 8_766 ?
Mo2 Mo4 Cs2 103.95(3) . 8_766 ?
Mo2 Mo4 Cs2 157.06(5) 7_565 8_766 ?
O13 Mo4 Cs2 67.1(4) . 2_655 ?
O14 Mo4 Cs2 36.6(3) 7_565 2_655 ?
O14 Mo4 Cs2 65.8(3) . 2_655 ?
O3 Mo4 Cs2 137.7(3) . 2_655 ?
O3 Mo4 Cs2 75.1(2) 7_565 2_655 ?
O1 Mo4 Cs2 145.51(13) . 2_655 ?
O8 Mo4 Cs2 117.3(2) . 2_655 ?
Mo2 Mo4 Cs2 157.06(5) . 2_655 ?
Mo2 Mo4 Cs2 103.95(3) 7_565 2_655 ?
Cs2 Mo4 Cs2 62.61(4) 8_766 2_655 ?
O13 Mo4 Cs3 130.4(5) . 2_664 ?
O14 Mo4 Cs3 34.8(3) 7_565 2_664 ?
O14 Mo4 Cs3 34.8(3) . 2_664 ?
O3 Mo4 Cs3 96.4(3) . 2_664 ?
O3 Mo4 Cs3 96.4(3) 7_565 2_664 ?
O1 Mo4 Cs3 127.8(3) . 2_664 ?
O8 Mo4 Cs3 55.0(3) . 2_664 ?
Mo2 Mo4 Cs3 124.53(4) . 2_664 ?
Mo2 Mo4 Cs3 124.53(4) 7_565 2_664 ?
Cs2 Mo4 Cs3 70.86(3) 8_766 2_664 ?
Cs2 Mo4 Cs3 70.86(3) 2_655 2_664 ?
O16 Mo5 O17 102.2(6) . 7_565 ?
O16 Mo5 O17 102.2(6) . . ?
O17 Mo5 O17 43.8(7) 7_565 . ?
O16 Mo5 O7 96.7(3) . . ?
O17 Mo5 O7 80.8(4) 7_565 . ?
O17 Mo5 O7 123.9(5) . . ?
O16 Mo5 O7 96.7(3) . 7_565 ?
O17 Mo5 O7 123.9(5) 7_565 7_565 ?
O17 Mo5 O7 80.8(4) . 7_565 ?
O7 Mo5 O7 148.1(5) . 7_565 ?
O16 Mo5 O2 100.5(6) . . ?
O17 Mo5 O2 148.2(4) 7_565 . ?
O17 Mo5 O2 148.2(4) . . ?
O7 Mo5 O2 74.6(3) . . ?
O7 Mo5 O2 74.6(3) 7_565 . ?
O16 Mo5 O6 173.6(6) . . ?
O17 Mo5 O6 83.7(5) 7_565 . ?
O17 Mo5 O6 83.7(5) . . ?
O7 Mo5 O6 81.7(3) . . ?
O7 Mo5 O6 81.7(3) 7_565 . ?
O2 Mo5 O6 73.1(4) . . ?
O16 Mo5 Mo3 90.6(4) . . ?
O17 Mo5 Mo3 114.4(4) 7_565 . ?
O17 Mo5 Mo3 156.4(4) . . ?
O7 Mo5 Mo3 33.6(3) . . ?
O7 Mo5 Mo3 117.6(3) 7_565 . ?
O2 Mo5 Mo3 43.26(6) . . ?
O6 Mo5 Mo3 84.7(2) . . ?
O16 Mo5 Mo3 90.6(4) . 7_565 ?
O17 Mo5 Mo3 156.4(4) 7_565 7_565 ?
O17 Mo5 Mo3 114.4(4) . 7_565 ?
O7 Mo5 Mo3 117.6(3) . 7_565 ?
O7 Mo5 Mo3 33.6(3) 7_565 7_565 ?
O2 Mo5 Mo3 43.26(6) . 7_565 ?
O6 Mo5 Mo3 84.7(2) . 7_565 ?
Mo3 Mo5 Mo3 84.76(5) . 7_565 ?
O16 Mo5 Cs2 45.3(3) . 5_655 ?
O17 Mo5 Cs2 89.9(3) 7_565 5_655 ?
O17 Mo5 Cs2 64.1(4) . 5_655 ?
O7 Mo5 Cs2 138.1(3) . 5_655 ?
O7 Mo5 Cs2 67.9(3) 7_565 5_655 ?
O2 Mo5 Cs2 121.9(2) . 5_655 ?
O6 Mo5 Cs2 138.08(15) . 5_655 ?
Mo3 Mo5 Cs2 134.55(5) . 5_655 ?
Mo3 Mo5 Cs2 85.18(4) 7_565 5_655 ?
O16 Mo5 Cs2 45.3(3) . 3_655 ?
O17 Mo5 Cs2 64.1(4) 7_565 3_655 ?
O17 Mo5 Cs2 89.9(3) . 3_655 ?
O7 Mo5 Cs2 67.9(3) . 3_655 ?
O7 Mo5 Cs2 138.1(3) 7_565 3_655 ?
O2 Mo5 Cs2 121.9(2) . 3_655 ?
O6 Mo5 Cs2 138.08(15) . 3_655 ?
Mo3 Mo5 Cs2 85.18(4) . 3_655 ?
Mo3 Mo5 Cs2 134.55(5) 7_565 3_655 ?
Cs2 Mo5 Cs2 71.27(5) 5_655 3_655 ?
O16 Mo5 Cs2 129.34(12) . 7_565 ?
O17 Mo5 Cs2 54.5(3) 7_565 7_565 ?
O17 Mo5 Cs2 88.8(4) . 7_565 ?
O7 Mo5 Cs2 41.4(3) . 7_565 ?
O7 Mo5 Cs2 133.9(3) 7_565 7_565 ?
O2 Mo5 Cs2 93.8(2) . 7_565 ?
O6 Mo5 Cs2 52.46(10) . 7_565 ?
Mo3 Mo5 Cs2 67.87(3) . 7_565 ?
Mo3 Mo5 Cs2 129.48(5) 7_565 7_565 ?
Cs2 Mo5 Cs2 143.89(4) 5_655 7_565 ?
Cs2 Mo5 Cs2 86.14(3) 3_655 7_565 ?
O9 Mn1 O9 94.3(5) . 7_575 ?
O9 Mn1 O12 173.7(4) . 7_575 ?
O9 Mn1 O12 85.8(4) 7_575 7_575 ?
O9 Mn1 O12 85.8(4) . . ?
O9 Mn1 O12 173.7(4) 7_575 . ?
O12 Mn1 O12 93.3(5) 7_575 . ?
O9 Mn1 O11 91.3(4) . . ?
O9 Mn1 O11 91.3(4) 7_575 . ?
O12 Mn1 O11 95.0(4) 7_575 . ?
O12 Mn1 O11 95.0(4) . . ?
O9 Mn1 O18 88.0(4) . . ?
O9 Mn1 O18 88.0(4) 7_575 . ?
O12 Mn1 O18 85.7(4) 7_575 . ?
O12 Mn1 O18 85.7(4) . . ?
O11 Mn1 O18 179.0(6) . . ?
O9 Mn1 Cs1 125.4(3) . 5_666 ?
O9 Mn1 Cs1 125.4(3) 7_575 5_666 ?
O12 Mn1 Cs1 50.6(3) 7_575 5_666 ?
O12 Mn1 Cs1 50.6(3) . 5_666 ?
O11 Mn1 Cs1 119.7(5) . 5_666 ?
O18 Mn1 Cs1 61.3(4) . 5_666 ?
O9 Mn1 Cs3 51.8(3) . . ?
O9 Mn1 Cs3 51.8(3) 7_575 . ?
O12 Mn1 Cs3 124.8(3) 7_575 . ?
O12 Mn1 Cs3 124.8(3) . . ?
O11 Mn1 Cs3 116.4(5) . . ?
O18 Mn1 Cs3 62.6(4) . . ?
Cs1 Mn1 Cs3 123.90(8) 5_666 . ?
O22 Cs1 O22 22(2) 7_565 . ?
O22 Cs1 O10 75.8(10) 7_565 7_565 ?
O22 Cs1 O10 89.2(10) . 7_565 ?
O22 Cs1 O10 89.2(10) 7_565 . ?
O22 Cs1 O10 75.8(10) . . ?
O10 Cs1 O10 76.2(4) 7_565 . ?
O22 Cs1 O12 132.8(10) 7_565 3_646 ?
O22 Cs1 O12 150.5(10) . 3_646 ?
O10 Cs1 O12 93.6(3) 7_565 3_646 ?
O10 Cs1 O12 133.3(3) . 3_646 ?
O22 Cs1 O12 150.5(10) 7_565 5_666 ?
O22 Cs1 O12 132.8(10) . 5_666 ?
O10 Cs1 O12 133.3(3) 7_565 5_666 ?
O10 Cs1 O12 93.6(3) . 5_666 ?
O12 Cs1 O12 60.8(4) 3_646 5_666 ?
O22 Cs1 O17 92.8(10) 7_565 7_566 ?
O22 Cs1 O17 88.0(10) . 7_566 ?
O10 Cs1 O17 153.5(3) 7_565 7_566 ?
O10 Cs1 O17 128.2(3) . 7_566 ?
O12 Cs1 O17 76.6(3) 3_646 7_566 ?
O12 Cs1 O17 62.7(3) 5_666 7_566 ?
O22 Cs1 O17 88.0(10) 7_565 1_556 ?
O22 Cs1 O17 92.8(10) . 1_556 ?
O10 Cs1 O17 128.2(3) 7_565 1_556 ?
O10 Cs1 O17 153.5(3) . 1_556 ?
O12 Cs1 O17 62.7(3) 3_646 1_556 ?
O12 Cs1 O17 76.6(3) 5_666 1_556 ?
O17 Cs1 O17 25.9(4) 7_566 1_556 ?
O22 Cs1 O18 155.4(10) 7_565 5_666 ?
O22 Cs1 O18 155.4(10) . 5_666 ?
O10 Cs1 O18 80.1(3) 7_565 5_666 ?
O10 Cs1 O18 80.1(3) . 5_666 ?
O12 Cs1 O18 53.3(2) 3_646 5_666 ?
O12 Cs1 O18 53.3(2) 5_666 5_666 ?
O17 Cs1 O18 111.3(3) 7_566 5_666 ?
O17 Cs1 O18 111.3(3) 1_556 5_666 ?
O22 Cs1 O15 92.1(10) 7_565 3_646 ?
O22 Cs1 O15 113.7(10) . 3_646 ?
O10 Cs1 O15 53.6(3) 7_565 3_646 ?
O10 Cs1 O15 127.6(3) . 3_646 ?
O12 Cs1 O15 48.7(2) 3_646 3_646 ?
O12 Cs1 O15 109.0(3) 5_666 3_646 ?
O17 Cs1 O15 104.1(3) 7_566 3_646 ?
O17 Cs1 O15 78.9(3) 1_556 3_646 ?
O18 Cs1 O15 77.47(18) 5_666 3_646 ?
O22 Cs1 O15 113.7(10) 7_565 5_666 ?
O22 Cs1 O15 92.1(10) . 5_666 ?
O10 Cs1 O15 127.6(3) 7_565 5_666 ?
O10 Cs1 O15 53.6(3) . 5_666 ?
O12 Cs1 O15 109.0(3) 3_646 5_666 ?
O12 Cs1 O15 48.7(3) 5_666 5_666 ?
O17 Cs1 O15 78.9(3) 7_566 5_666 ?
O17 Cs1 O15 104.1(3) 1_556 5_666 ?
O18 Cs1 O15 77.47(18) 5_666 5_666 ?
O15 Cs1 O15 154.0(4) 3_646 5_666 ?
O22 Cs1 Mn1 164.1(10) 7_565 5_666 ?
O22 Cs1 Mn1 164.1(10) . 5_666 ?
O10 Cs1 Mn1 106.6(2) 7_565 5_666 ?
O10 Cs1 Mn1 106.6(2) . 5_666 ?
O12 Cs1 Mn1 32.52(18) 3_646 5_666 ?
O12 Cs1 Mn1 32.52(18) 5_666 5_666 ?
O17 Cs1 Mn1 78.3(2) 7_566 5_666 ?
O17 Cs1 Mn1 78.3(2) 1_556 5_666 ?
O18 Cs1 Mn1 33.9(2) 5_666 5_666 ?
O15 Cs1 Mn1 77.69(17) 3_646 5_666 ?
O15 Cs1 Mn1 77.69(17) 5_666 5_666 ?
O7 Cs2 O16 103.9(3) 7_565 5_655 ?
O7 Cs2 O14 169.2(3) 7_565 8_755 ?
O16 Cs2 O14 65.4(3) 5_655 8_755 ?
O7 Cs2 O6 55.7(3) 7_565 . ?
O16 Cs2 O6 150.5(3) 5_655 . ?
O14 Cs2 O6 133.1(3) 8_755 . ?
O7 Cs2 O19 116.9(3) 7_565 8_755 ?
O16 Cs2 O19 139.1(4) 5_655 8_755 ?
O14 Cs2 O19 73.7(3) 8_755 8_755 ?
O6 Cs2 O19 64.1(4) . 8_755 ?
O7 Cs2 O17 46.6(3) 7_565 . ?
O16 Cs2 O17 98.1(3) 5_655 . ?
O14 Cs2 O17 130.3(3) 8_755 . ?
O6 Cs2 O17 52.5(3) . . ?
O19 Cs2 O17 107.1(4) 8_755 . ?
O7 Cs2 O4 51.3(2) 7_565 . ?
O16 Cs2 O4 138.3(3) 5_655 . ?
O14 Cs2 O4 138.0(2) 8_755 . ?
O6 Cs2 O4 48.8(3) . . ?
O19 Cs2 O4 76.2(3) 8_755 . ?
O17 Cs2 O4 86.3(2) . . ?
O7 Cs2 O11 93.4(3) 7_565 1_545 ?
O16 Cs2 O11 87.6(3) 5_655 1_545 ?
O14 Cs2 O11 88.2(3) 8_755 1_545 ?
O6 Cs2 O11 112.6(3) . 1_545 ?
O19 Cs2 O11 93.0(4) 8_755 1_545 ?
O17 Cs2 O11 139.9(3) . 1_545 ?
O4 Cs2 O11 64.8(2) . 1_545 ?
O7 Cs2 O17 56.2(3) 7_565 5_655 ?
O16 Cs2 O17 49.4(3) 5_655 5_655 ?
O14 Cs2 O17 113.7(3) 8_755 5_655 ?
O6 Cs2 O17 111.3(3) . 5_655 ?
O19 Cs2 O17 168.8(3) 8_755 5_655 ?
O17 Cs2 O17 75.0(3) . 5_655 ?
O4 Cs2 O17 93.1(2) . 5_655 ?
O11 Cs2 O17 79.3(3) 1_545 5_655 ?
O7 Cs2 O7 68.2(3) 7_565 3_645 ?
O16 Cs2 O7 46.5(2) 5_655 3_645 ?
O14 Cs2 O7 101.6(2) 8_755 3_645 ?
O6 Cs2 O7 104.0(3) . 3_645 ?
O19 Cs2 O7 148.9(4) 8_755 3_645 ?
O17 Cs2 O7 52.0(2) . 3_645 ?
O4 Cs2 O7 119.1(2) . 3_645 ?
O11 Cs2 O7 117.8(3) 1_545 3_645 ?
O17 Cs2 O7 40.4(2) 5_655 3_645 ?
O7 Cs2 O20 103.6(3) 7_565 . ?
O16 Cs2 O20 127.3(3) 5_655 . ?
O14 Cs2 O20 85.2(3) 8_755 . ?
O6 Cs2 O20 81.0(3) . . ?
O19 Cs2 O20 47.4(4) 8_755 . ?
O17 Cs2 O20 132.9(3) . . ?
O4 Cs2 O20 52.8(2) . . ?
O11 Cs2 O20 46.8(3) 1_545 . ?
O17 Cs2 O20 123.2(3) 5_655 . ?
O7 Cs2 O20 163.5(2) 3_645 . ?
O7 Cs2 Mo5 80.85(17) 7_565 5_655 ?
O16 Cs2 Mo5 23.2(3) 5_655 5_655 ?
O14 Cs2 Mo5 88.4(2) 8_755 5_655 ?
O6 Cs2 Mo5 129.9(2) . 5_655 ?
O19 Cs2 Mo5 161.3(3) 8_755 5_655 ?
O17 Cs2 Mo5 80.3(2) . 5_655 ?
O4 Cs2 Mo5 121.92(16) . 5_655 ?
O11 Cs2 Mo5 91.6(2) 1_545 5_655 ?
O17 Cs2 Mo5 28.85(17) 5_655 5_655 ?
O7 Cs2 Mo5 29.39(14) 3_645 5_655 ?
O20 Cs2 Mo5 138.01(19) . 5_655 ?
O15 Cs3 O15 79.8(4) 5_666 3_656 ?
O15 Cs3 O14 105.7(3) 5_666 8_766 ?
O15 Cs3 O14 87.9(3) 3_656 8_766 ?
O15 Cs3 O14 87.9(3) 5_666 2_665 ?
O15 Cs3 O14 105.7(3) 3_656 2_665 ?
O14 Cs3 O14 27.7(4) 8_766 2_665 ?
O15 Cs3 O9 77.2(3) 5_666 . ?
O15 Cs3 O9 113.7(3) 3_656 . ?
O14 Cs3 O9 158.2(3) 8_766 . ?
O14 Cs3 O9 134.1(3) 2_665 . ?
O15 Cs3 O9 113.7(3) 5_666 7_575 ?
O15 Cs3 O9 77.2(3) 3_656 7_575 ?
O14 Cs3 O9 134.1(3) 8_766 7_575 ?
O14 Cs3 O9 158.2(3) 2_665 7_575 ?
O9 Cs3 O9 58.2(4) . 7_575 ?
O15 Cs3 O19 162.9(4) 5_666 7_575 ?
O15 Cs3 O19 112.2(4) 3_656 7_575 ?
O14 Cs3 O19 87.3(4) 8_766 7_575 ?
O14 Cs3 O19 99.7(3) 2_665 7_575 ?
O9 Cs3 O19 86.7(4) . 7_575 ?
O9 Cs3 O19 60.2(3) 7_575 7_575 ?
O15 Cs3 O19 112.2(4) 5_666 . ?
O15 Cs3 O19 162.9(4) 3_656 . ?
O14 Cs3 O19 99.7(3) 8_766 . ?
O14 Cs3 O19 87.3(4) 2_665 . ?
O9 Cs3 O19 60.2(3) . . ?
O9 Cs3 O19 86.7(4) 7_575 . ?
O19 Cs3 O19 53.6(7) 7_575 . ?
O15 Cs3 O18 62.1(3) 5_666 . ?
O15 Cs3 O18 62.1(3) 3_656 . ?
O14 Cs3 O18 148.6(3) 8_766 . ?
O14 Cs3 O18 148.6(3) 2_665 . ?
O9 Cs3 O18 52.1(2) . . ?
O9 Cs3 O18 52.1(2) 7_575 . ?
O19 Cs3 O18 111.6(3) 7_575 . ?
O19 Cs3 O18 111.6(3) . . ?
O15 Cs3 O10 51.6(3) 5_666 . ?
O15 Cs3 O10 128.3(3) 3_656 . ?
O14 Cs3 O10 118.3(3) 8_766 . ?
O14 Cs3 O10 90.7(3) 2_665 . ?
O9 Cs3 O10 46.3(2) . . ?
O9 Cs3 O10 104.5(2) 7_575 . ?
O19 Cs3 O10 112.6(4) 7_575 . ?
O19 Cs3 O10 60.9(3) . . ?
O18 Cs3 O10 78.35(17) . . ?
O15 Cs3 O10 128.3(3) 5_666 7_575 ?
O15 Cs3 O10 51.6(3) 3_656 7_575 ?
O14 Cs3 O10 90.7(3) 8_766 7_575 ?
O14 Cs3 O10 118.3(3) 2_665 7_575 ?
O9 Cs3 O10 104.5(2) . 7_575 ?
O9 Cs3 O10 46.3(2) 7_575 7_575 ?
O19 Cs3 O10 60.9(3) 7_575 7_575 ?
O19 Cs3 O10 112.6(4) . 7_575 ?
O18 Cs3 O10 78.35(17) . 7_575 ?
O10 Cs3 O10 150.6(3) . 7_575 ?
O15 Cs3 O16 55.3(2) 5_666 5_666 ?
O15 Cs3 O16 55.3(2) 3_656 5_666 ?
O14 Cs3 O16 58.0(3) 8_766 5_666 ?
O14 Cs3 O16 58.0(3) 2_665 5_666 ?
O9 Cs3 O16 131.9(2) . 5_666 ?
O9 Cs3 O16 131.9(2) 7_575 5_666 ?
O19 Cs3 O16 141.3(4) 7_575 5_666 ?
O19 Cs3 O16 141.3(4) . 5_666 ?
O18 Cs3 O16 94.6(3) . 5_666 ?
O10 Cs3 O16 99.77(15) . 5_666 ?
O10 Cs3 O16 99.77(15) 7_575 5_666 ?
Mo4 O1 Mo2 98.8(3) . . ?
Mo4 O1 Mo2 98.8(3) . 7_565 ?
Mo2 O1 Mo2 150.1(6) . 7_565 ?
Mo4 O1 Mo1 99.6(5) . . ?
Mo2 O1 Mo1 100.3(3) . . ?
Mo2 O1 Mo1 100.3(3) 7_565 . ?
Mo5 O2 Mo3 96.5(3) . . ?
Mo5 O2 Mo3 96.5(3) . 7_565 ?
Mo3 O2 Mo3 155.4(6) . 7_565 ?
Mo5 O2 Mo1 99.4(5) . . ?
Mo3 O2 Mo1 99.1(3) . . ?
Mo3 O2 Mo1 99.1(3) 7_565 . ?
Mo2 O3 Mo4 109.3(4) . . ?
Mo1 O4 Mo3 112.3(4) . 7_565 ?
Mo1 O4 Mo2 111.9(4) . 7_565 ?
Mo3 O4 Mo2 91.7(3) 7_565 7_565 ?
Mo1 O4 Cs2 96.9(3) . . ?
Mo3 O4 Cs2 89.9(3) 7_565 . ?
Mo2 O4 Cs2 148.0(4) 7_565 . ?
Mo2 O5 Mo3 114.5(4) . . ?
Mo1 O6 Mo5 105.4(6) . . ?
Mo1 O6 Cs2 107.7(2) . 7_565 ?
Mo5 O6 Cs2 91.2(3) . 7_565 ?
Mo1 O6 Cs2 107.7(2) . . ?
Mo5 O6 Cs2 91.2(3) . . ?
Cs2 O6 Cs2 142.5(4) 7_565 . ?
Mo3 O7 Mo5 111.0(4) . . ?
Mo3 O7 Cs2 116.8(4) . 7_565 ?
Mo5 O7 Cs2 112.3(4) . 7_565 ?
Mo3 O7 Cs2 117.4(4) . 3_655 ?
Mo5 O7 Cs2 82.7(3) . 3_655 ?
Cs2 O7 Cs2 111.8(3) 7_565 3_655 ?
Mo1 O8 Mo4 106.1(6) . . ?
Mo1 O8 Cs3 161.2(6) . 2_664 ?
Mo4 O8 Cs3 92.7(4) . 2_664 ?
Mo2 O9 Mn1 141.7(5) . . ?
Mo2 O9 Cs3 112.4(4) . . ?
Mn1 O9 Cs3 96.8(3) . . ?
Mo2 O10 Cs1 133.3(5) . . ?
Mo2 O10 Cs3 96.6(4) . . ?
Cs1 O10 Cs3 118.1(3) . . ?
Mn1 O11 Cs2 112.1(5) . 7_565 ?
Mn1 O11 Cs2 112.1(5) . 1_565 ?
Cs2 O11 Cs2 80.8(3) 7_565 1_565 ?
Mo3 O12 Mn1 144.3(5) . . ?
Mo3 O12 Cs1 109.8(4) . 5_666 ?
Mn1 O12 Cs1 96.9(3) . 5_666 ?
O14 O14 Mo4 67.7(3) 7_565 . ?
O14 O14 Cs3 76.2(2) 7_565 2_664 ?
Mo4 O14 Cs3 124.0(4) . 2_664 ?
O14 O14 Cs2 120.4(2) 7_565 8_766 ?
Mo4 O14 Cs2 121.5(5) . 8_766 ?
Cs3 O14 Cs2 113.3(3) 2_664 8_766 ?
Mo3 O15 Cs3 145.2(6) . 5_666 ?
Mo3 O15 Cs1 94.1(4) . 5_666 ?
Cs3 O15 Cs1 120.6(3) 5_666 5_666 ?
Mo5 O16 Cs2 111.5(4) . 5_655 ?
Mo5 O16 Cs2 111.5(4) . 3_655 ?
Cs2 O16 Cs2 99.3(4) 5_655 3_655 ?
Mo5 O16 Cs3 128.7(6) . 5_666 ?
Cs2 O16 Cs3 100.9(3) 5_655 5_666 ?
Cs2 O16 Cs3 100.9(3) 3_655 5_666 ?
O17 O17 Mo5 68.1(4) 7_565 . ?
O17 O17 Cs1 77.0(2) 7_565 1_554 ?
Mo5 O17 Cs1 140.5(6) . 1_554 ?
O17 O17 Cs2 134.5(2) 7_565 . ?
Mo5 O17 Cs2 97.8(4) . . ?
Cs1 O17 Cs2 93.5(3) 1_554 . ?
O17 O17 Cs2 116.54(19) 7_565 5_655 ?
Mo5 O17 Cs2 87.1(4) . 5_655 ?
Cs1 O17 Cs2 126.0(3) 1_554 5_655 ?
Cs2 O17 Cs2 105.0(3) . 5_655 ?
Mn1 O18 Cs1 84.8(4) . 5_666 ?
Mn1 O18 Cs3 84.5(4) . . ?
Cs1 O18 Cs3 169.3(4) 5_666 . ?
Cs2 O19 Cs3 158.2(6) 8_766 . ?
O22 O22 Cs1 79.2(10) 7_565 . ?
 
_refine_diff_density_max    5.727
_refine_diff_density_min   -4.579
_refine_diff_density_rms    0.443



